to-metal transition occurs (open squares). The opposite phase transition (metal-to-insulator) can be observed in \[fig:CurrentMIT\_IR\_ins\] upon decreasing current, as indicated by the open diamonds. We note that the square and diamond markers lie, within our experimental resolution, within the ranges of $\Tim$ and $\Tmi$, respectively. This indicates that the current-driven MIT is triggered whenever the local temperature of an area goes above $\Tim$ or below $\Tmi$. The experimental setup used in the present work does not allow us to detect additional non-thermal effects induced by the electrical current, which may have caused changes in $\Tim$ and $\Tmi$ smaller than our uncertainty of.

Current-driven MIT in the presence of cracks and defects
--------------------------------------------------------

To study how the formation of cracks and defects affects the current-driven MIT, we perform multiple current cycles that bring the sample to the metallic state and then back to the insulating state. The thermal bath is fixed at $\Tp=\SI{25}{\celsius}$. The current is increased up to a few larger than what required to switch the entire sample to the metallic phase, and then decreased back to zero (rates of ). We show in \[fig:Fatigue\_V,fig:Fatigue\_A\] the two-probe $V$–$I$ characteristics and value of $\Ai$ measured during nine consecutive cycles. At each cycle, the voltage peak increases and shifts to lower currents (triangles in \[fig:Fatigue\_V\]) and to lower corresponding current densities ($\jp$ in \[fig:Fatigue\_j\]). Concomitantly, the entire sample turns metallic at a lower current (stars in \[fig:Fatigue\_A\]) and current density ($\ja$ in \[fig:Fatigue\_j\]). This occurs because a higher power is dissipated in the sample due to its increased resistance. The drop of more than one order of magnitude in $\ja$ indicates large and irreversible changes in the sample properties, consistent with the previous observation of crack formation at similar current values.

The formation of cracks and defects strongly affects the temperature distribution over the sample surface, leading to the formation of hot spots responsible for higher power dissipation, as can be seen in the images of \[fig:Fatigue\_imgs\]. It is clear that, despite the comparable values of $\Ai$, the presence of hot spots in the lower left (right) corner during the 2nd (8th)
to - metal transition occurs (open public square). The diametric phase transition (metal - to - insulator) can be note in \[fig: CurrentMIT\_IR\_ins\ ] upon decrease current, as indicated by the open diamond. We notice that the square and diamond markers lie, within our experimental resolution, within the range of $ \Tim$ and $ \Tmi$, respectively. This indicates that the current - driven MIT is triggered whenever the local temperature of an area goes above $ \Tim$ or below $ \Tmi$. The experimental setup use in the present work does not allow us to detect additional non - thermal effect induced by the electrical current, which may have caused change in $ \Tim$ and $ \Tmi$ smaller than our uncertainty of. 

 Current - driven MIT in the presence of cracks and defect 
 -------------------------------------------------------- 

 To study how the formation of cracks and defects affects the current - driven MIT, we perform multiple current cycles that bring the sample to the metallic state and then back to the insulating state. The thermal bath is fixed at $ \Tp=\SI{25}{\celsius}$. The current is increased up to a few larger than what necessitate to switch the entire sample distribution to the metallic phase, and then decrease back to zero (rate of). We show in \[fig: Fatigue\_V, fig: Fatigue\_A\ ] the two - probe $ V$–$I$ characteristic and value of $ \Ai$ measured during nine consecutive cycles. At each cycle, the electric potential peak increases and shifts to lower currents (triangles in \[fig: Fatigue\_V\ ]) and to lower corresponding current densities ($ \jp$ in \[fig: Fatigue\_j\ ]). Concomitantly, the entire sample turns metallic at a gloomy current (star in \[fig: Fatigue\_A\ ]) and current density ($ \ja$ in \[fig: Fatigue\_j\ ]). This occurs because a higher power is dissipated in the sample distribution due to its increased resistance. The drop of more than one order of magnitude in $ \ja$ indicates large and irreversible changes in the sample property, consistent with the former observation of crack formation at similar current values. 

 The constitution of cracks and defect strongly involve the temperature distribution over the sample surface, precede to the formation of blistering spots responsible for higher office dissipation, as can be seen in the images of \[fig: Fatigue\_imgs\ ]. It is clear that, despite the comparable values of $ \Ai$, the bearing of hot spots in the low left (right) corner during the 2nd (8th )
to-mftal transition occurs (oken squares). The okpisite 'hase tdansitiov (metal-to-insulator) can be obdeeved un \[fig:CurrentMIT\_IR\_ins\] jpon decrvasing cuerenu, as indicated by the opek diajlnds. Xe note that thg square and diamond markess lne, within our experimental resolutiog, withim hhe ranges of $\Jim$ amq $\Tmj$, respectively. This indicates that the cugrent-driven MIT ix triggered whenever the llcal temperature of an area goes qbovq $\Tim$ or belod $\Tmi$. The tx'erimental aetup used in the present work aoes uot allow uw ro fgtect additiinal gon-thermal engects hnduced by the electrlcal rurrwnt, which may have cansed changes in $\Tim$ wnd $\Tmi$ skamler than our uncwrrainti of.

Cgrrevr-drkveh KIF in tje 'resence of cracks and defects
--------------------------------------------------------

To study hoe eye formation kf craskf and defects affects the current-driven MIF, we perform multiple cyrrent cycles that brlng the swmple to the metallic state and then back to the hnsuletkng sbate. Rhf thermal bath is fixed at $\Tp=\SI{25}{\celsius}$. The cuwdemt is increased mp to a few larger tjam what requirea to scjtdh the entire samppe to tre merallic phwse, snd then decreased back to zero (rates oy ). Qe show in \[fig:Fatiyue\_V,fig:Fatigbe\_A\] thg two-ptobe $V$–$I$ characteristics and value of $\Al$ measures during nine conrecltiva cycles. At each cycle, the voltage 'eak nncreaser anc shifes to loweg curvants (triangles in \[vig:Fajigue\_V\]) and to loaer corresponding current densivmes ($\jp$ in \[fig:Gadigle\_j\]). Concoiitanbly, the entire fample turns mgtallic ac a loder currenn (stars ii \[fig:Fatigue\_W\]) and current fensity ($\ja$ ii \[fig:Fatidue\_j\]). Thiw occurr because a higner power is dissipqted in the sample dug fo its increaseb twsistance. The croo os loce thwt one order mf mxgnkyude kn $\ja$ indicctds lsrge and irreversibla chznges in the samplr iropertiew, consiseent with the previous observatlon oh cracy forkatyon at similar current values.

Tge formatlon of cracks agd dcfecjs strongly affects the temperature distribution oter the sample surface, oeading to the formctlon of hot s'ots rqsponsibla for higher power dussipation, as can be seen in the imagea of \[fhg:Fatlgue\_imgs\]. It is clear that, despite the comparable values of $\Ai$, the presencw of hot spots in fhe kower lzft (right) coriec during the 2nd (8tn)
to-metal transition occurs (open squares). The opposite (metal-to-insulator) be observed \[fig:CurrentMIT\_IR\_ins\] upon decreasing open We note that square and diamond lie, within our experimental resolution, within ranges of $\Tim$ and $\Tmi$, respectively. This indicates that the current-driven MIT is whenever the local temperature of an area goes above $\Tim$ or below $\Tmi$. experimental used the work does not allow us to detect additional non-thermal effects induced by the electrical current, which have caused changes in $\Tim$ and $\Tmi$ smaller our uncertainty of. Current-driven in the presence of cracks defects To study the of and defects affects current-driven MIT, we perform multiple current cycles that bring the sample to the metallic state and then to the The thermal is at The current is to a few larger than what the entire sample to the metallic phase, and decreased back zero (rates of ). We show \[fig:Fatigue\_V,fig:Fatigue\_A\] the two-probe $V$–$I$ characteristics and value of measured during nine consecutive cycles. At each cycle, the voltage peak increases and shifts to (triangles in \[fig:Fatigue\_V\]) and lower corresponding current ($\jp$ \[fig:Fatigue\_j\]). the sample turns at a lower current (stars in \[fig:Fatigue\_A\]) and current density ($\ja$ \[fig:Fatigue\_j\]). This occurs because a higher power is dissipated in due its increased resistance. drop of more than order magnitude in $\ja$ indicates irreversible in consistent the observation of crack formation similar current values. The formation cracks and defects strongly the sample surface, leading to the formation of spots responsible for higher power dissipation, as be seen in the images of \[fig:Fatigue\_imgs\]. It is clear that, despite comparable values the presence of hot spots in the lower (right) corner during the (8th)
to-metal transition occurs (opEn squares). THe oppOsiTe pHaSe trAnsiTion (metal-to-insULatoR) can be observed in \[fig:CurRentMiT\_ir\_ins\] UPoN decrEasing cURrENT, as InDiCatEd BY tHe opeN diAmonds. WE note that tHe sQuAre and diamonD MaRkers lie, wiThiN our experimeNtaL resolUtIon, WIthin The RangeS of $\Tim$ ANd $\Tmi$, rEspectiveLy. tHis indICates thAT ThE curRent-driven MIT is trIGgERed whenever the Local tEmPErATUre Of aN area goes aBoVe $\Tim$ OR below $\TMI$. THE EXpeRImental setup uSed in the preSEnt Work doEs Not ALlow us To detEcT AddItional non-tHermAl effects InduceD By the elECtrical CurrenT, whIch May hAVe CaUseD cHAngES iN $\TiM$ And $\tmi$ smallEr ThAn our UnceRTAINty oF.

CuRrenT-drivEn MIT in the preSenCe of CRacKs and DefecTs
--------------------------------------------------------

To StUdy hoW the foRmatiOn Of cracks and defeCts aFfects the CurReNt-dRiVen MIt, We perfOrm MulTiple cuRrent cyCLes ThAT BRiNg the sample to the meTaLLIc State and Then baCK tO tHE insulatInG stAte. THE ThermAl baTH iS fixed at $\tp=\SI{25}{\ceLSiUs}$. the currEnT is incReAseD up To a feW LargEr than What requIred tO Switch the entirE Sample to the meTAlLIC pHAse, aNd tHen decreaseD bacK To zeRo (raTEs Of ). WE Show iN \[fig:FAtIGuE\_v,fig:Fatigue\_A\] the two-pRoBe $V$–$I$ chAractEristics and vaLue of $\Ai$ meaSUREd during Nine COnSEcutive cycles. AT each Cycle, the voLTage peak IncreAses and sHifts to loWER currentS (trIanGleS in \[FIG:FAtigue\_V\]) and to lOWEr coRrEspondiNg cUrrent dEnsItiEs ($\jP$ in \[FiG:Fatigue\_j\]). concomitAnTlY, tHe EntIre saMPle turns MeTalLiC at A loweR CurrenT (starS in \[fIg:faTIguE\_A\]) and cuRReNT DensItY ($\jA$ in \[fIg:FAtIgue\_j\]). this OCcuRs becauSe a higher PowER is dIsSiPated in The sample due tO iTs increaseD rEsiStance. tHE drop of mOre than one order of magnitUDe in $\ja$ iNdiCates LargE and irrevErsIble chAngES in the Sample PropeRtIes, CONsistENT wIth ThE previous oBSErvAtion Of CracK formatIon at similar currenT ValUes.

The formatiOn oF craCKS aNd dEFeCTs sTrONglY AFfects the temperAture distrIbUTiOn over the sAMplE sUrface, lEading tO the fORmation Of hot spotS responsiBlE for HIGheR power dissIpation, aS can be seeN In the IMaGes of \[Fig:fatiguE\_iMgs\]. it is cLear thAT, deSpite The comPaRable vAlues Of $\ai$, the preSence of hot spots in the lowEr left (Right) CorNer during The 2ND (8th)
to-metal transition occurs  (open squ ares) . T heop posi te p hase transitio n  (me tal-to-insulator) canbe ob se r vedi n\[fig :Curren t MI T \ _IR \_ in s\]  u p on  decr eas ing cur rent, as i ndi ca ted by the o p en  diamonds.  We  note that t hesquare  a ndd iamon d m arker s lie, within  our expe ri m entalr esoluti o n ,with in the ranges of$ \T i m$ and $\Tmi$,  respe ct i ve l y . T his  indicates  t hat t h e curre n t- d r i ven MIT is trigge red wheneve r  th e loca ltem p eratur e ofan are a goes abov e $\ Tim$ or b elow $ \ Tmi$. T h e exper imenta l s etu p us e din  th ep res e nt  wo r k d oes notal lo w usto d e t e c t ad dit iona l non -thermal effe cts  ind u ced  by t he el ectr ic al cu rrent,  whic hmay have caused  cha nges in $ \Ti m$  an d$\Tmi $  small ertha n our u ncertai n tyof . Cu rrent-driven MIT i nt h epresence  of cr a ck sa nd defec ts 
-- ---- - - ----- ---- - -- -------- ------ - -- -- ------- -- ------ -- 

T o s tudyh ow t he for mation o f cra c ks and defects affects the c u rr e n t- d rive n M IT, we perf ormm ulti plec ur ren t  cycl es th at br i ng the sample to th emetall ic st ate and thenback to th e i nsulatin g st a te .  The thermal b ath i s fixed at $\Tp=\SI {25}{ \celsius }$. The c u r rent isinc rea sed  up t oa few largert h an w ha t requi red  to swi tch  th e e nti re  sample t o the me ta ll ic  p has e, an d  then de cr eas ed  ba ck to zero ( rates  of).  W e  sh ow in \ [ fi g : Fati gu e\ _V,f ig: Fa tigue \_A\ ]  th e two-p robe $V$– $I$ char ac te ristics  and value of  $ \Ai$ measu re d d uringn i ne conse cutive cycles. At eachc ycle, t hevolta ge p eak incre ase s andshi f ts tolowercurre nt s ( t r iangl e s  i n \ [f ig:Fatigue \ _ V\] ) and  t o lo wer cor responding current den sities ($\jp$  in  \[f i g :F ati g ue \ _j\ ]) .  Co n c omitantly, theentire sam pl e  t urns metal l icat  a lowe r curre nt (s t ars in\[fig:Fat igue\_A\] )andc u rre nt density  ($\ja$in \[fig: F atigu e \_ j\]).  Th is occ ur s b ecaus e a hi g her  powe r is d is sipate d inth e sample  due to its increased r esista nce.The  drop ofmor e  th an one or derof magnitu dein$\ja$  in d icate s la r ge  an d  irre vers i ble chang e sint h esample prop e r t ies , con sis t ent wi th t he previous obser v ation of crack  for m a tio n a t  sim il ar current val ues .T he forma ti on of crack s and de fe c ts st rongly  affec ts thet e mp e rature  dis tri bution ov erth e  sample  s ur f ace, l eadi ng  to th e form a tion o f hot spots resp onsib l e  forh igh er po we r dissi p atio n, as canbe seen inthe im ages  of \ [fig:Fa ti gue\_i mgs \] . It is cl e ar that,despi te theco mpar abl e valu es o f $\Ai$ , th epre sence ofh o ts po ts inthelower  l eft(right) c o rner dur ing the 2nd  ( 8th ) 
to-metal transition_occurs (open_squares). The opposite phase_transition (metal-to-insulator)_can_be observed_in_\[fig:CurrentMIT\_IR\_ins\] upon decreasing_current, as indicated_by the open diamonds._We note that_the_square and diamond markers lie, within our experimental resolution, within the ranges of $\Tim$_and_$\Tmi$, respectively._This_indicates_that the current-driven MIT is_triggered whenever the local temperature_of an_area goes above $\Tim$ or below $\Tmi$. The_experimental_setup used in_the present work does not allow us to detect_additional non-thermal effects induced by the_electrical current, which_may_have_caused changes in $\Tim$_and $\Tmi$ smaller than our uncertainty_of.

Current-driven MIT in the presence of_cracks and defects
--------------------------------------------------------

To study how the formation_of cracks and defects affects the_current-driven MIT, we perform multiple_current cycles_that bring the sample to_the metallic state_and then_back to the_insulating state. The thermal bath is_fixed at $\Tp=\SI{25}{\celsius}$._The current is increased up to_a_few larger than_what_required_to switch_the entire sample_to_the metallic_phase,_and then decreased back to zero_(rates_of ). We show in \[fig:Fatigue\_V,fig:Fatigue\_A\] the_two-probe $V$–$I$ characteristics and_value_of $\Ai$ measured during_nine consecutive cycles. At each_cycle, the voltage peak increases and_shifts to_lower currents_(triangles in \[fig:Fatigue\_V\]) and to lower corresponding current densities ($\jp$ in_\[fig:Fatigue\_j\]). Concomitantly, the entire sample turns_metallic at a lower_current (stars_in_\[fig:Fatigue\_A\]) and current_density_($\ja$ in_\[fig:Fatigue\_j\]). This occurs because a higher power_is dissipated_in the sample due to its_increased resistance. The drop_of_more than one order of magnitude_in $\ja$ indicates large and irreversible_changes in the sample properties,_consistent_with_the previous observation of crack_formation at similar current values.

The formation_of cracks and_defects strongly affects the temperature distribution over_the_sample surface, leading to the formation_of_hot spots responsible for higher power_dissipation,_as_can be seen in the_images of \[fig:Fatigue\_imgs\]. It is clear_that, despite the comparable values of $\Ai$, the presence_of hot spots_in the lower left (right)_corner_during_the 2nd (8th)